*e-mail: benedito@dee.ufcg.edu.br

**Nanocrystalline Material in Toroidal Cores for Current Transformer: **

**Analytical Study and Computational Simulations **

**Benedito Antonio Luciano****a _{*, João Marcelo Cavalcante de Albuquerque}a**

_{, }**Walman Benício de Castro****b _{, Conrado Ramos Moreira Afonso}c**
a

_{Department of Electrical Engineering, CEEI/UFCG, }

_{Department of Electrical Engineering, CEEI/UFCG, }

*P. B. 10105, 58109 970 Campina Grande - PB, Brazil *

b

_{Department of Mechanical Engineering, CCT/UFCG, }

_{Department of Mechanical Engineering, CCT/UFCG, }

*58109-970 Campina Grande - PB, Brazil *

c

_{Materials Engineering, Pos-Graduate Program in Materials Science Engineering, UFSCar, }

_{Materials Engineering, Pos-Graduate Program in Materials Science Engineering, UFSCar, }

*Via Washington Luís, km 235, 13565-905 São Carlos - SP, Brazil*

*13565-905 São Carlos - SP, Brazil*

Received: July 19, 2004; Revised: October 19, 2005

Based on electrical and magnetic properties, such as saturation magnetization, initial permeability, and coercivity, in this work are presented some considerations about the possibilities of applications of nanocrystalline alloys in toroidal cores for current transformers. It is discussed how the magnetic characteristics of the core material affect the performance of the current transformer. From the magnetic characterization and the computational simulations, using the finite element method (FEM), it has been verified that, at the typical CT operation value of flux density, the nanocrystalline alloys properties reinforce the hypothesis that the use of these materials in measurement CT cores can reduce the ratio and phase errors and can also improve its accuracy class.

**Keywords: ***nanocrystalline alloys, toroidal cores, current transformer*

**1. Introduction**

Current transformer (CT) is an instrument transformer specially designed and assembled to be used in measurement, control, and protective circuits. Its primary circuit consists of a few turns – some-times even a single turn – and is connected in serie with the circuit whose current is desired to be measured, and the secondary circuit is connected to the current-measuring instruments.

The theory about CT is basically the same of any other iron-core transformer. The secondary circuit is closed through the typical low impedance of the instruments connected to it. Normally, these are 5 A instruments. The voltage across the secondary terminals is the drop through the instruments and loads, and usually is only a few volts. The voltage across the primary terminals is approximately the voltage referred to the primary, and can be only a fraction of a volt.

In the ideal CT, the secondary current is inversely proportional to the ratio of turns and oppositive in phase to the impressed primary current. However, an exact inverse proportionality and phase relation are not possible because part of the primary current must be used to excite the magnetic material of the core. So, the exciting current must be subtracted phasorially from the primary current to find the amount remaining to supply secondary current. This value will be slightly different from the value that the ratio of turns would indicate and there is a slight shift in the phase relationship. This results in the introduction of ratio and phase angle errors when compared to the ideal CT.

Since the exciting current alters the ratio and phase angle of the primary and secondary currents, it is made as small as possible through the use of high permeability and low loss magnetic materials in the construction of the core, such as silicon steel and amorphous

alloys. In many industrial applications, designers need to select the
magnetic core material and its shape. Each specific application
de-mands the development of a specific core shape. Therefore, they all
have advantages and drawback; for instance, toroidal cores are more
compact than E-cores and their material cost is lower due to single
component and tighter magnetic coupling1_{.}

In this work, it is presented a study about the possibilities of application of nanocrystalline alloys in toroidal cores for current transformers.

**2. Analytical Study and Some **

**Design Considerations**

Current transformers are characterized by some relationships.
The first is the marked ratio of the primary current to the secondary
current (*K _{c}* =

*I*), and is indicated by the manufacturer. This ratio is a fixed and permanent value for a given current transformer. The second is the true ratio of the rms primary current to the rms second-ary current (

_{pn }/ I_{sn}*K*=

_{r}*I*/

_{p }*I*) under specified conditions. The true ratio of a current transformer is not a single fixed value, since it depends on the specified conditions of use, such as secondary burden (

_{s}*Z*), primary current (

_{c}*I*), frequency (

_{p}*f*), and wave form. The third is the ratio cor-rection factor (RCF). It is the factor by which the marked ratio must be multiplied to obtain the true ratio (RCF =

*K*/

_{r }*K*).

_{c}these considerations, Figure 1 can represent the CT electrical model,
where *Z _{s}* is the secondary impedance.

*2.1. Phase angle*

The phase angle of a current transformer, designated by the
Greek letter b, is the angle between the current leaving the
identi-fied secondary terminal and the current entering the identiidenti-fied
primary terminal, under specified conditions2_{. It is apparent from }
Figure 2 that the reversed secondary current *I _{2}* is not in phase
with the impressed primary current

*I*, there is an angle between them, the phase angle b. This angle is considered positive when the secondary current leads the primary current and it is usually expressed in minutes.

_{1}In this Figure, φ is the magnetizing flux and *I _{0}* is the exciting
current with its two components:

*I*

_{µ}, the magnetizing current, and

*I*, the active losses current. In the secondary circuit:

_{p}*E*is the induced electromotive force,

_{2}*r*is the winding resistance,

_{2}*x*is the leakage reactance,

_{2}*U*is the terminal voltage,

_{2}*I*is the secondary current, and θ

_{2}*2*is the angle between

*U2*and

*I*2. In addition, it can be seen that the primary current

*I*is obtained by phasor sum of

_{1}*I*and (–

_{0}*n*/

_{2 }*n*).

_{1}*I*, where

_{2}*n*and

_{2}*n*are the number of turns of the secondary and primary windings, respectively.

_{1}*2.2. The influence of the primary and the secondary currents *

*on the CT errors*

The ratio error ε* _{c}*is defined as the percent relative difference
be-tween the measured value of the primary current and its exact value,
as expressed by the equation:

.

. %

*I*

*K I* *I* _{100}

*c*
*r*

1

2 1

f= - (1)

On the other hand, the phase angle error is defined as the angle b presented on the phasor diagram of the CT in Figure 2.

The main reason for the ratio and phase angle errors of a current
transformer is the exciting current *I _{0}*. In an ideal TC, in which

*I*does not exist,

_{0}*I1*and – (

*n*/

_{2 }*n*).

_{1}*I2*presented in Figure 2 are coincident. Thus, the primary current value, obtained from the secondary current, would be equal to the absolute value of the vector

*I1*from the phasor diagram, and this vector would be delayed from

*I2*of exactly 180°.

In conventional transformers, the exciting current is considered constant, and its absolute value and phase can be determined by open-circuit test. However, this is not true in CT. In a current transformer the exciting current is not constant, neither in its absolute value nor in its phase, due to the great influence of the non-linearity of the magnetic material of which its core is made. Due to the relation between the primary and the exciting currents, the smaller the value of the first one, the greater the influence of the second, what increases the ratio and phase angle errors of the CT. That is why, when determining the accuracy class of a CT, the technical norms allow the CT to present bigger errors when tested with 10% of the primary nominal current than when it is tested with its exact value.

Analysing Figure 2, it can be verified the influence of the exciting
and the primary currents on the errors of a CT. In this figure, projecting
the vectors *Io* and *I2* over the vector *I1*, it is obtained:

. .cos .cos ( )

*I*1 =*Kc* *I*2 b+ *Io* 790c- a+b+d A (2)

where α is the angle between the exciting current *Io* and the
mag-netizing flux z, and δ is the angle between the inverse of *I2* and the
inverse of *E2*.

Due to its relatively small value, the angle b can be neglected, simplifying the previous expression:

*Zm* *Zc*

*ZS*

*Is*

*Ie*

*Ip*

**Figure 1.** Equivalent electric circuit of a current transformer.

*I1*

*I*_{M}
*Io*

*I2*

*U2*

*E2*

*X2I2*

*Ip*

B

90°

Q2 Q0

F
-*n _{n}2*

*1I2*

**Figure 2.** Phasor diagram of a current transformer.

. .sen( )

*I*1 =*Kc* *I*2 + *Io* a+b & (3)

.sen( )

*I*

*K I* *I*

*I*
*I*

*c* *o*

1

2 1

1

& - =- a+d

Analysing the second equality of expression (3), it can be seen that its first member is equal to the ratio error of the CT, which will be considered in its absolute value in a new expression:

.

.sen( ) .sen( )

*I*

*K* *I* *I*

*I*
*I*

*I*
*I*

*c* *o*

*c*
*o*

1

2 1

1 1

&

a d f a d

-=- + = + (4)

Again from the phasor diagram of Figure 2, the follow expression for the tangent of the angle b can be obtained:

. .

. ( )

cos sen

*tg*

*K* *I*

*I* 90

*c*
*o*

2

c b

b a b d

= 7 - + + A (5)

Considering that the angle b has a relatively small value, a simpler expression can be, then, obtained:

.cos( )

*I*
*Io*

1

b= a+d (6)

primary current decreases. Then, it is important that the magnetic material of the CT core could demand a small exciting current to be magnetized and, also, that the CT could be projected to operate with a primary current value as near as possible of its nominal value, in order to minimize the effects of the primary current in its errors.

In turn, the secondary current of a CT is extremely dependent of its primary current, and it is not influenced by the impedance of the element connected to the secondary terminals of the CT. However, if this impedance exceeds some limit values, determined by the maxi-mum power with which the accuracy class of the CT was obtained, the errors can be much greater than those obtained with the tests.

When an impedance *Z* is connected to the secondary of a CT, a
current *I _{2}* flows through it and the ratio and phase angle errors ε

*and b, respectively, can be determined by Equations 4 and 6. When the absolute value of*

_{c}*Z*increases, keeping its phase unchanged, it is nec-essary an increase of the secondary voltage

*U*so that the secondary current

_{2}*I*could stay constant. To achieve this aim, the electromotive force

_{2}*E*has to increase its absolute value and so on the flux ϕ inside the core. As this flux is produced by the exciting current

_{2}*I*, it must also increase its absolute value, increasing the ratio and phase angle errors. This analysis of the influence of the secondary current on the CT errors is important, because it alerts about the resistance limit of the conductors that could be used to connect the secondary windings of the CT to the equipments that they will supply.

_{o}*2.3. Some design considerations*

An essential part of the transformer design consists of the
deter-mination of the magnetic cross-section area (*A _{mag}*) and the conductors
cross-section area. These areas are determined from estimations of
suitable values for the peak flux density

*B*; the full-load rms current density

_{m}*J*in the windings, that depends on the way transformers will be used, intermittently or continuously; the winding space factor

*k*; and the stacking factor

_{w}*k*.

_{s}The primary and secondary windings must be accommodated in
the window area *A _{w}*. The winding space factor

*k*is defined as the ratio between the total conductor cross-section area and the window area. Insulation and clearance reduce the available area for actual conductor cross-section to

_{w}*k*.

_{w}*A*. The full-load rms current density in the windings

_{w}*J*is limited by

*r*.

*I*2

_{ loss and heat dissipation. The stacking }factor

*k*is defined as the ratio between the magnetic cross-section area and the total core cross-section area.

_{s}As nanocrystalline materials are produced in the form of ribbons, it is available toroidal cores with square or rectangular cross-section, as shown in Figure 3.

The dimensioning of the magnetic circuit starts with the deter-mination of the magnetic cross-section area, given by:

*A _{mag }= k_{S}.A_{geo}* (7)

where *A _{geo}* is the geometric cross-section area.

The medium length of the magnetic circuit is given by:

*lmag*=r *OD*_{2} *ID*

+

b l (8)

The number of each winding turns *N* is obtained by the
equa-tion:

. . .

*N*

*k f B A*
*V*

*f* *m* *mag*

= (9)

where *V* is the rated rms voltage, *f* is the frequency of the signals,
and *k _{f}* is the form factor (equal to 4.44 for sine wave and equal to
4.0 for square wave).

The cross-section areas of the two windings, the primary (*A _{p}*) and
secondary (

*A*), are determined considering the full-load rms current density in the winding and the work rate of the transformer, by the following relationships:

_{s}.

*A*
*J V*

*S*
*p*

1

= (10)

.

*A*
*J V*

*S*
*s*

2

= (11)

Because of the m.m.f. balance (*N _{1}*.

*I*=

_{1 }*N*.

_{2}*I*), each one of the primary and secondary windings occupy about one-half of the avail-able area, so that the primary current linkage is

_{2}*N*.

_{1}*I*=

_{1 }*(1/2)*.

*k*.

_{w}*A*.

_{w}*J*

and the rms value of the current is given by:

. . .

*I*

*N*
*k A J*

2

*rms*

*w* *w*

= (12)

where *A _{w}* is the geometrical core window area and

*k*is the winding factor.

_{w}By Faraday’s law, for sinusoidal wave, the rms value of the voltage is:

*V _{rms }= *4.44.

*f*.

*N*.

*A*.

_{mag}*B*(13)

_{m}Therefore, as *V _{rms }*=

*S/I*, the transformer volt-ampere rating is given by:

_{rms}*S* = 2.22.*f*.*B _{m}*.

*J*.

*K*.

_{w}*A*.

_{w}*A*(14)

_{mag}It is shown in Equation 14 that the transformer volt-ampere
rating is proportional to the product of the available window area
of the core multiplied by the magnetic cross-section area, which
is called area product. There is a unique relationship between this
area product, characteristic value for transformer cores, and several
other important parameters that must be considered in transformers
design, such as volume, weight, surface area and current density, for
a given temperature rise3_{.}

Using Ampère’s law, and considering the total m.m.f. for a peak
flux density as *H _{m}l_{mag}*, where

*l*is the mean length of the flux path around the magnetic circuit, the magnetizing current

_{mag}*I*in the

_{m}*N*turns of the primary windings, ignoring harmonics, is given by:

_{1}. .

*I*

*N*
*H l*

2

*m*
*m* *mag*

1

= (15)

**3. Nanocrystaline Alloys Development**

The first nanocomposite soft magnetic alloy based on the
Fe-Cu-M(-Si)-B alloy (M: Nb, Mo, Ta, W, Zr, etc.) was obtained by
Yoshizawa et al.4_{. The first step was to produce amorphous metal }
ribbons of about 20 µm thickness. Next, the amorphous ribbons were
wound into toroidal cores, and then the core materials were annealed
to produce the nanocrystalline soft magnetic material with an average
grain size of approximately 10 nm5_{. }

After Yoshizawa et al. report4_{, nanocrystalline materials have }
been investigated for applications in magnetic devices requiring
OD

HT

ID

OD = Outer diameter ID = Inner diameter HT = Height

both magnetically hard and soft materials. In particular, amorphous
and nanocrystalline alloys have been used as the core material in
some electromagnetic devices, such as distribution transformers,
common mode choke coils, pulse transformers, impulse current
transformers, transformers for switched-mode power supplies and
current transformers6_{.}

**4. Magnetic Characterization**

In Figures 4, 5 and 6 are presented the hysteresis curve at 60 Hz, the permeability curve at 60 Hz and the initial magnetization curve at 5 Hz, obtained for the nanocrystalline alloy FINEMET® FT-3M F6045G produced by Hitachi Metals Ltd.

From the magnetic characterization, it has been verified that, to the typical CT operation value of 0.2 T, the nanocrystalline properties reinforce the hypothesis that the use of these materials in measurement CT cores can reduce both the relation and phase errors and can also improve its accuracy class.

**5. Numerical Calculation Using FEMM Package**

Whilst analytical method is useful for must problems
concern-ing transformers design, the numerical methods provide a better
understanding of transformers electromagnetic behavior. Indeed,
numerical methods, such as the finite element method, allow an
ac-curate determination of flux densities in the whole domain and also
the study of local phenomena. In this work, a finite element method
computer program was carried out in order to obtain the flux density
inside the magnetic material in the toroidal core CT previously
de-signed. These simulations were performed using the electromagnetic
package FEMM 3.3 applied for low frequencies7_{.}

In the simulations, a quarter of the toroidal core was chosen as the domain of study, as this part of the entire geometry presents symmetry along the horizontal and vertical axies. This proceeding helps to re-duce the processing time needed. The program FEMM 3.3 was used to simulate the behaviour of a CT whose electrical and magnetic circuits were previously designed by analytical proceedings. Four simulations were realized, which aimed to compare the CT performance when its core was composed of four different magnetic materials.

The magnetic materials chosen to be compared as the CT core material were: the nanocrystalline alloy FINEMET® FT-3M F6045G, produced by the Japanese company Hitachi Metals Ltd.; the amor-phous alloy METGLAS® 2605S-2, produced by the American compa-ny Honeywell International; the nanocrystalline alloy NANOPERM® M-033-03 N1, produced by the German company Magnetec GmbH; and grain oriented (GO) silicon-iron E-004, produced by the Brasil-ian company Acesita.

In Table 1 there are some magnetic characteristics of the magnetic
materials studied in the simulations. Silicon steel is an example of
magnetic material commonly used in the cores of commercial CT.
Thus, the simulations could compare the performance between
fer-rocrystalline conventional materials and new magnetic materials as
CT cores. In this table, *B _{s}* is the saturation flux density, µ

*is the maximum value of the relative permeability, and ρ is the resistivity of the material.*

_{rmax}A CT is used in such a way that the magnitude of secondary cur-rent has negligible influence on magnitude of the primary curcur-rent. Thus, as the primary winding gives the necessary energy to the core magnetization, it was the only one winding designed in simulations. Its eight turns were uniformly distributed along the core and just two of then appear in the quarter designed. The conductor used in the primary winding is made of copper and, according to the previous calculations, has the diameter of the wire 5 AWG. To design the core, it was used the real dimensions of the magnetic material and of the

- 50 - 40 - 30 - 20 - 10 0 10 20 30 40 50 Magnetic Field H (A/m)

Magnetic Induction B (T)

1.0

0.2

0.6

0.4

0.2

0.0

- 0.2

- 0.4

- 0.6

- 0.2

- 1.0 FINEMET Alloy 60 Hz

**Figure 4.** Hysteresis curve at 60 Hz.

FINEMET Alloy 60 Hz

0 5 10 15 20 25 30 35 40 45 50 55 60 Magnetic Field H (A/m)

200,000

175,000

150,000

125,000

100,000

75,000

50,000

25,000

0

Relati

ve Permeability (

M

)

**Figure 5.** Magnetic permeability curve at 60 Hz.

0 5 10 15 20 25 30 35 40 45 50

Magnetic Field H (A/m) 2.00

1.75

1.50

1.25

1.00

0.75

0.50

0.25

0.00

Magnetic Induction B (T)

FINEMET Alloy 5 Hz

**Figure 6.** Initial magnetization curve at 5 Hz.

capsule of non-magnetic material that envolves the core FINEMET® FT-3M F6045G. The domain of study divided in the finite elements of the mesh is shown in Figure 7.

material that would occupy the place in the domain reserved to the
core. From the resuts given by the program, some informations
were collected for each one of the magnetic materials studied.
These data were: the magnetic field intensity (*H*) in the place of
the core where the magnetic induction reached the desired value
of 0.2 T; the relative magnetic permeability (µ* _{R}*) at this point; and
the excitation current (

*I*) necessary to obtain that operation induc-tion value. In Table 2 can be seen these values obtained for every magnetic material studied.

_{o}In Figure 8 is shown one of the graphics provided by FEMM 3.3 for the simulation using the nanocrystalline alloy FINEMET® FT-3M F6045G. The magnetic flux lines stay confined within the magnetic material of the core, due to its high relative permeability value in comparison with the others elements of the domain. The intensity of

the magnetic flux can be observed by the colour scale in the figure, where the more intense is the red tinge, the greater is the flux density in the material.

The calculations show that the field and flux density vary ra-dially in a wound toroid. In each simulation, the copper turns of the primary winding conducted the calculated value of exciting current necessary to induce inside each magnetic material a mean flux density of 0.2 T. To reach this particular value of magnetic induction in the core, the nanocrystalline alloy FINEMET® FT-3M F6045G was the magnetic material that demanded the lowest value of exciting current, followed by the amorphous alloy METGLAS® 2605S-2. Their values of exciting currents are extremely lower than the one demanded by the GO silicon-iron E-004, which does not present a high magnetic permeability at the CT operation induc-tion value. Finally, the other nanocrystalline alloy, NANOPERM® M-033-03 N1, although presenting very low rates of magnetic losses at 60 Hz, also needed a relatively high value of exciting current. This alloy congregates good magnetic properties in general, but particularly at 0.2 T your relative magnetic permeability is very lower than that presented by the nanocrystalline alloy FINEMET® FT-3M F6045G.

**6. Conclusions**

From the magnetic characterization and the computational simulations, using the finite element method (FEM), it has been verified that, at the typical current transformers operation value of 0.2 T, the nanocrystalline alloys properties reinforce the hypothesis that the use of these materials in measurement current transformer cores can reduce the relation and phase errors and can also improve its accuracy class.

**Acknowledgments**

The authors are grateful to Hitachi Metals Ltd. and Magnetec GmbH for providing the nanocrystalline alloys in toroidal cores shape, and to ACESITA and TOROID for the important informations con-ceded. The present investigation was sponsored by PROCAD/CAPES – 0104/01-9 and CNPq.

**Table 1.** Magnetic materials simulated as CT cores.

Material Composition *B _{s}* (T) (60 Hz) µ

*(60 Hz) ρ (µΩ.m)*

_{rmax}FINEMET® FT-3M F6045G Fe_{73,5}Cu_{1}Nb_{3}Si_{13,5}B_{9} 0.90 185,000 (3.0 A.m-1_{)} _{1.20}
NANOPERM® M-033-03 N1 Fe_{73,5}Si_{15,5}Cu_{1}Nb_{3}B_{7} 1.18 34,985 (1.8 A.m-1_{)} _{1.15}

METGLAS® 2605S-2 Fe_{78}Si_{9}B_{13} 1.56 193,397 (4.3 A.m-1_{)} _{1.37}

Silicon-iron GO E-004 Fe-3.2%Si 1.85 40,154 (23.0 A.m-1_{)} _{0.47}

**Table 2.** Parameters obtained for each magnetic material by simulation.

Magnetic Material Values Obtained by Simulation for 0.2 T and 60 Hz

*H* (A.m-1_{)} µ

R *Io* (mA)

FINEMET® FT-3M F6045G 1.46 109,100 31.34

NANOPERM® M-033-03 N1 5.43 29,270 110.70

METGLAS® 2605S-2 1.64 97,090 34.82

Silicon-iron GO E-004 6.93 22,930 141.36

Air

Air

Air

Air CooperExt

FINEMET FT-3M F6045G

CooperExt

Copperlnt Copperlnt

45 G

2.658e-001 : > 2.797e-001 2.518e-001 : 2.658e-001 2.378e-001 : 2.518e-001 2.238e-001 : 2.378e-001 2.098e-001 : 2.238e-001 1.958e-001 : 2.098e-001 1.819e-001 : 1.958e-001 1.679e-001 : 1.819e-001 1.539e-001 : 1.679e-001 1.399e-001 : 1.539e-001 1.259e-001 : 1.399e-001 1.120e-001 : 1.259e-001 9.797e-002 : 1.120e-001 8.399e-002 : 9.797e-002 7.000e-002 : 8.399e-002 5.602e-002 : 7.000e-002 4.204e-002 : 5.602e-002 2.806e-002 : 4.204e-002 1.407e-002 : 2.806e-002 < 9.184e-005: 1.407e-002 Density Plot: |B|, Tesla

**Figure 8.** Scale of flux density in the elements of the domain.

**References**

1. Luciano BA, Guimarães MKA, Castro WB. Journal of metastable and
nanocrystalline materials. In: Kiminami, CK, Botta Filho WJ, guest
edi-tors. *Some designs considerations on industrial applications of amorphous *

*and nanocrystalline alloys*. *Proceedings of the 1st _{ Workshop on Metastable }*

*and Nanostrutured Materials*; 2001 August 16-17; *São Pedro, SP, Brazil*.

Switzerland: Trans Tech Publications. 2002. p. 133-138.

2. Edison Electric Institute. *Electrical Metermen´s Handbook*. Seventh
Edition. New York: EEI: 1965.

3. McLyman, CWT. *Magnetic core selection for transformers and inductors: *

*a user’s guide to practice and specification*. New York: Marcel Dekker:

1997.

4. Yoshizawa Y, Oguma S, Yamauchi K. New Fe-based soft magnetic alloys
composed of ultrafine grain structure. *Journal of Applied Physics*. 1988;
64(1):6044-6046.

5. Yoshizawa Y. Magnetic properties and microstructure of nanocrystalline
Fe-based alloys. *Journal Metastable and Nanocrystalline Materials*. 1999;
1(1):51-62.

6. Mchenry ME, Laughlin DE. Nano-scale materials development for future
magnetic applications. *Acta Materialia*. 2000; 48(1):223-238.